Detailed EL performances of di-chromatic WOLED devices discussed in this chapter are summarized in Table 3-3. It is apparent that introducing p-i-n
system into OLED device architecture can indeed reduce the drive voltage. To carefully control the RZ location in a thin layer thickness, we demonstrated highly efficient p-i-n WOLEDs with a DEML system, in which the co-deposited NPB molecules in the DEML were used as the assistant dopant (NPB) to shift the RZ towards the blue emitting layer and balance the blue and yellow emission intensity. The refined exciton confinement of p-i-n WOLED device III has been shown to significantly improve the EL performance, giving rise to 10 cd/A and 9.3 lm/W at 1000 cd/m2 and a stable white color under various drive conditions.
Table 3-3 EL performances of WOLED devices at 20 mA/cm2
We also developed a tandem p-i-n WOLED device IV consists of two individual p-i-n WOLED units connected electrically with an optical transparent and doped organic p-n junction utilizing BPhen: Cs2CO3/NPB: WO3. The charge-carriers for recombination of this tandem WOLED are well-balanced under various current densities due to the DEML system in each individual p-i-n WOLED, giving rise to one of the best EL efficiency of 23.9 cd/A and 7.8 lm/W with CIEx,y coordinates of (0.30, 0.43). The EL color of the tandem device IV will not change significantly with respect to drive current variation and forward viewing angle.
really has the potential to be applied in portable electronics due to its high power efficiency. In addition, WOLEDs with tandem structure also can be one candidate of solid-state light source due to its high brightness at low current density. However, these di-chromatic WOLEDs still have drawbacks, such as low color gamut about 61-62% and low CRI value of 67. These undesirable properties will affect their applications in full-color display and light source.
Therefore, to improve the color gamut and CRI value, our experiments will focus on developing tri-chromatic WOLED device in next chapter.
 Commission internationale de l'Eclairage proceedings, Cambridge:
Cambridge University Press (1931).
 G. B. Rybicki, A. P. Lightman, Radiative Processes in Astrophysics, New York: John Wiley & Sons (1979).
 J. Mehra, H. Rechenberg, The Historical Development of Quantum Theory, 1, New York: Springer-Verlag (1982).
 G. Wyszelki, W. S. Siles, Color Science, 2nd edition, New York: Wiley (1982).
 A. R. Duggal, J. J. Shiang, C. M. Heller, D. F. Foust, Appl. Phys. Lett. 80, 3470 (2002).
 J. Kido, K. Hongawa, K. Okuyama, K. Nagei, Appl. Phys. Lett. 64, 815 (1994).
 J. Kido, M. Kimura, K. Nagei, Science 267, 1332 (1995).
 R. F. Service, Science 310, 1762 (2005).
 B. W. D’Andrade, S. R. Forrest, Adv. Mater. 16, 1585 (2004).
 I. ul Haq Raja, J. Y. Lee, I. T. Kim, S. H. Lee, Monatsh. Chem. 139, 725 (2005).
 K. T. Kamtekar, A. P. Monkman, M. R. Bryce, Adv. Mater. 22, 572 (2010).
 P. A. Levermore, V. Adamovich, K. Rajan, W. Yeager, C. Lin, S. Xia, G. S.
Kottas, M. S. Weaver, R. Kwong, R. Ma, M. Hack, J. J. Brown, Proceedings of
SID2010, p. 786, May 23-28 (2010), Seattle, WA, USA.
 P. Loebl, V. van Elsbergen, H. Boerner, C. Goldmann, S. Grabowski, D.
Bertram, Proceedings of SID2010, p. 782, May 23-28 (2010), Seattle, WA, USA.
 T. Komoda, H. Tsuji, N. Ito, T. Nishimori, N. Ide, Proceedings of SID2010, p. 993, May 23-28 (2010), Seattle, WA, USA.
 M. T. Lee, H. H. Chen, C. H. Tsai, C. H. Liao, C. H. Chen, Appl. Phys. Lett.
85, 3301 (2004).
 Y. Sato, Semicond. Semimetals 64, 209 (2000).
 H. Murata, C. D. Merritt, Z. H. Kafafi, IEEE J. Sel. Top. Quantum Electron.
4, 119 (1998).
 J. Huang, M. Pfeiffer, A. Werner, J. Blochwitz, S. Liu, K. Leo, Appl. Phys.
Lett. 80, 139 (2002).
 C. H. Kim and J. Shinar, Appl. Phys. Lett. 80, 2201 (2002).
 J. T. Lim, N. H. Lee, Y. J. Ahn, G. W. Kang, C. H. Lee, Curr. Appl. Phys. 2, 295 (2002).
 P. M. Borsenberger, L. Pautmeier, R. Richert, Bässler, J. Chem. Phys. 94, 8276 (1991).
 T. Yasuda, Y. Yamaguchi, D. C. Zou, T. Tsutsui, Jpn. J. Appl. Phys. Part 1
41, 5626 (2002).
 C. C. Chang, M. T. Hsieh, J. F. Chen, S. W. Hwang, C. H. Chen, Appl. Phys.
Lett. 89, 253504 (2006).
 B. Wei, K. Furukawa, M. Ichikawa, T. Koyama, Y. Taniguchi, Mol. Cryst.
Liq. Cryst. 426, 295 (2005).
 Y. S. Wu, T. H. Liu, H. H. Chen, C. H. Chen, Thin Solid Films 496, 626 (2006).
 L. S. Liao, K. P. Klubek, C. W. Tang, Appl. Phys. Lett. 84, 167 (2004).
 T. Y. Cho, C. L. Lin, C. C. Wu, Appl. Phys. Lett. 88, 111106 (2006).
 C. C. Chang, J. F. Chen, S. W. Hwang, C. H. Chen, Appl. Phys. Lett. 87, 253501 (2005).
 F. Guo and D. Ma, Appl. Phys. Lett. 87, 173510 (2004).
 V. Bulovic, V. B. Khalfin, G. Gu, P. E. Burrows, D. Z. Garbuzov, S. R.
Forrest, Phys. Rev. B 58, 3730 (1998).
 J. S. Kim, P. K. H. Ho, N. C. Greenham, R. H. Friend, J. Appl. Phys.88, 1073 (2000).
 K. Saxena, D. S. Mehta, R. Srivastava, M. N. Kamalasanan, Appl. Phys.
Lett. 89, 061124 (2006).
Development of Fluorescent Deep Blue System and Tri-Chromatic White Organic Light-Emitting Diodes
For full-color OLED display applications, it is essential to deliver a set of primary RGB emitters with sufficiently high luminous efficiency, properly balanced color chromaticity, as well as sufficient operational stability. Such a set of emitters has been amply demonstrated by using a guest-host doped emitting system which encompasses a single or cohost matrix dispersed with various highly fluorescent or phosphorescent guest dopants leading to EL with the desirable hues . With the discovery and rapid improvement of phosphorescent dopant materials along with their matching host, hole-blocker and device architecture capable of harvesting both the singlet and triplet excitons electro-generated in the doped emitter, in today’s OLEDs, to achieve high efficiency and color saturation for the red and green emitters is no longer a major problem. The decision by Pioneer in 2003 announcing the use of one of United Display Corporation’s (UDC) red phosphorescent dopants coupled with a BAlq-based host material in its new 1.1-in passive matrix 96 RGB 72 full-color subdisplay cellular phone has all but removed the last skepticism hanging over the intrinsic stability issue of phosphorescent materials worthy of production . In 2009, UDC disclosed their improvement for red phosphorescent devices (26 cd/A) with operational stability of 500000 h at an initial luminance of 1000 cd/cm2 and CIEx,y coordinates close to (0.24, 0.36) .
Similar improvement of extremely efficient green phosphorescent devices (64
cd/A) with operational stability of 150000 h at an initial luminance of 1000 cd/cm2 and CIEx,y coordinates close to (0.35, 0.61) has also been achieved by UDC . It is expected that, in the future, we would also find one of these red and green phosphorescent materials ending up in some forms of OLED products in the marketplace.
Unfortunately, the same cannot be said for the state-of-the-art of the phosphorescent blue emitter which remains to be the weakest link in the development of RGB phosphorescent materials. At the International Display Manufacturing Conference (IDMC) 2005, held in Taipei, Taiwan, Samsung SDI managed to disclose for the first time  a deep blue phosphorescent emitter with (0.15, 0.15) but only can last for 150 h. To date, the best triplet blue emitter reported is due to UDC  which claimed to have achieved a luminous efficiency of about 69 cd/A at 1000 cd/m2 with a sky blue emission at wavelength of 474 nm, unfortunately, there is no lifetime data for this new blue emitter. Part of the problems in producing a decent saturated blue phosphorescent emitter is due to the fact that there is simply no good host material available that possesses sufficiently large triplet bandgap energy (3 eV) to effectively prevent triplet exciton of the dopant from quenching by back energy transfer, and the limitation of short-conjugated ligand selection for synthesizing transition metal-based metal–ligand charge-transfer (MLCT) complexes serves only to compound the already grave and aggravated situation . All things considered, it suffices to predict that the advent of a robust phosphorescent blue emitter with all of the necessary attributes for high efficiency, saturated color, as well as device stability would be extremely difficult.
Recently, several approaches to high-efficiency WOLEDs have been demonstrated, foremost among them introduces a blue fluorescent dopant together with red and green phosphorescent dopants in the emission layer (EML) [7,8]. In that device, the blue fluorescent dopant harvests a majority of singlet excitons, with the remainder of lower energy triplets diffusing through the conductive host to directly excite the green and red phosphors. This architecture allows for increased power efficiency by resonant energy transfer from the conductive host into both the singlet and triplet energy levels. Indeed, this architecture eliminates exchange energy losses of 0.5-1.0 eV resulting from intersystem crossing from the host singlet into a blue phosphor triplet state.
It is mainly for this reason that developing fluorescent blue OLEDs with high efficiency, deep-blue color, and long operational lifetime is indispensable and is always being considered. There have been many reports on blue host materials have been reported, such as anthracene (will be introduced in next section), di(styryl)arylene , tetra(phenyl)pyrene , terfluorenes [11,12], and tetra(phenyl)silyl derivatives [13,14].
In this chapter, we design and develop a new blue anthracene-based host for fluorescent deep blue emitter and adopt this efficient deep blue system into
tri-chromatic WOLED device architecture.
4.2 Prominent blue fluorescence OLED materials based on anthracene core structure
Anthracene has a rigid ring structure that minimizes vibronic energy levels to give very high fluorescence quantum efficiency as well as color purity. In addition, chemical modification of anthracene is relatively easier than most other rigid aromatics due to its better solubility in common organic solvents.
Furthermore, anthracene possesses 14-electron aromaticity, thus it is relatively stable in terms of thermal and electrochemical properties. However, anthracene by itself with no substituent attached is highly crystalline, fluoresces in the near UV and has a propensity to crystallize in thin-films, which greatly limits its application in OLED. Therefore, various studies have been focused on derivatizing anthracene core with aromatic substituents on 9-, 10- and/or bulky steric substituents on 2-, 6- positions as shown in Figure 4-1 to prevent its crystallization and stabilize its thin-film morphology upon thermal evaporation into thin-films. One of the best deep blue fluorescent derivative among these is 9,10- diphenylanthracene known as DPA which has near unity fluorescence quantum efficiency in dilute solution and is also highly fluorescent in the solid state. But its fluorescence is too deep in the blue and it is prone to crystallize in solid-state thin film [15,16], thereby limiting its OLED applications. This is because crystalline formation in solid-state device destroys thin-film homogeneity, creates pin-holes and raises electrical resistance that ultimately leads to device failure . It is well known that amorphous thin film materials as applied to OLEDs having high Tg are almost always less vulnerable to heat and, hence, their devices perform more stably [18,19,20,21]. Thus, there have been numerous anthracene derivatives designed and synthesized with strategically positioned bulky groups which were beneficial to stabilize their amorphous solid-state by virtue of their dissymmetrical molecular shape that mitigates intermolecular interaction and crystal formation. Later, studies also showed that the introduction of bulky spacer can alleviate unfavorable excimer emission .
Figure 4-1 Structures of anthracene-based blue host materials.
In 2002, Shi and Tang at Kodak reported the first stable blue OLED emitter using 2, 5, 8, 11-tetra(t-butyl)perylene (TBP) blue dopant and 9,10-di(2-naphthyl)anthracene (ADN) as blue host material. Their device structure was ITO/copper phthalocyanine (CuPc) (25 nm)/NPB (50 nm)/ADN:TBP (30 nm)/Alq3 (40 nm)/Mg:Ag (9:1, 200 nm), which achieved a luminance efficiency of 3.5 cd/A with CIEx,y coordinates of (0.15, 0.23). The device operational lifetime reported was about 4000 hrs with an initial luminance of 636 cd/m2, which was the best ever published in a formal journal and a blue OLED record of its time.
After the disclosure of this pioneering report, many researchers started to focus and pursue materials based on anthracene with better, hopefully improved EL performance than that of ADN. It was soon discovered that the morphology of thin-film ADN as blue host material is unstable and tends to deteriorate
(crystallize) under prolonged electrical stress or annealing at elevated temperatures (95 °C), and its blue EL color is also not pure with CIEx,y of (0.17, 0.17) . Quickly, in attempts to improve the emissive color, the tert-butyl substituted derivative at
C-2position of anthracene namely, 2-(t-butyl)-9,10-di(2-naphthyl)anthracene (TBADN), was reported by the Kodak group in an European patent . Using the same dopant and device configuration, TBADN was able to generate a deeper blue emission of CIEx,y
(0.13, 0.19), but its efficiency was considerably lower than that of ADN, and unfortunately neither morphological nor device stability data was disclosed in that patent.
In 2004, two isomeric anthracene derivatives, 2,3,6,7-tetramethyl-9,10-di(1-naphthyl) anthracene (-TMADN) and 2,3,6,7-tetramethyl-9,10-di(2-naphthyl) anthracene (-TMADN) were reported to provide highly efficient blue emission with similar design concept [26,27]. In the device structure of ITO/NPB (50 nm)/blue emitter (15 nm)/4,7-diphenyl-1,10-phenanthroline (BPhen, 40 nm)/Mg:Ag,
-TMADNdevice achieved a current efficiency of 3.1 cd/A with CIEx,y of (0.15, 0.21). The efficiency of -TMADN was better with 4.5 cd/A and CIE coordinates of (0.16, 0.22). The experimental results clearly demonstrated that the introduction of four methyl groups to the molecular structure of ADN appears to be beneficial in producing improved device performance. The reason may be that the twisted nonplanar molecular structures of -TMADN and -TMADN which is distorted by the steric effect of the four methyl substituents could prevent the undesirable molecular aggregation . Additionally, it was revealed that when the blend of
-TMADN and -TMADN was used as the light-emitting material, the device
performance can be further improved to 5.2 cd/A with CIEx,y of (0.15, 0.23). The improved efficiency was attributed to the higher fluorescent quantum yield of
-TMADN. (The fluorescence quantum yields of -TMADN and -TMADNwere measured to be 0.50 and 0.65, respectively.)
In an effort to improve the thin-film morphological stability of ADN by molecular engineering, several multi-t-butyl-substituted ADN derivatives, such as 2,6-di(t-butyl)-9,10-di(2-naphthyl)anthracene (DTBADN) and 2,6-di(t-butyl)-9,10-di[6-(t-butyl)-2-naphthyl]anthracene (TTBADN) were synthesized and compared with ADN and TBADN  (structures are shown in Figure 4-1). It was discovered, however, by virtue of its inductive effect, that the
t-butyl groups could induce significant bathochromic shift of ADN’sfluorescence in both of these derivatives and consequently lower its PL quantum efficiency. It was also suggested that the greenish color and low EL efficiency of DTBADN and TTBADN could be due to the bulky t-butyl groups which tend to twist the chromophore of ADN as revealed by computer simulations using the Quantum CAChe (v. 5.02) program.
To search for derivatives of ADN without adversely impacting on its EL emission, efficiency and charge-carrier mobility, a systematic study of alkyl substitution on the 2-position of ADN was launched in our lab. It was found that the best way to stabilize the morphology of ADN was to strategically place a relatively small methyl-group at C-2 position of the anthracene moiety, MADN, which can readily be synthesized by Suzuki coupling of the 2-methyl-9,10-dibromo-anthracene with 2-(napthyl)boronic acid according to a known procedure . By computer simulation, it was found that the symmetry and close molecular packing of ADN is disrupted by the methyl substituent
which results in the increase of the intermolecular distance. As a result, the thin-film surface morphology of MADN is considerably more robust than that of ADN as revealed by the AFM photographs before and after annealing (as shown in Figure 4-2). The small methyl substituent imparts no effect on the LUMO/HOMO level of ADN which remains at 2.5/5.5 eV with a bandgap energy of 3 eV. Table 4-1 compares the solution PLs of various substituted ADN derivatives in toluene along with its thermal properties. In comparison with their solution PL fluorescence and relative quantum efficiency in toluene, both MADN and TBADN have better efficiency than those of ADN.
Low-temperature PL studies revealed also that both MADN and TBADN have different vibronic levels which hypsochromic-shift their luminescence peaks significantly enough that their CIE color coordinates move to deeper blue and therefore have potential for deep blue OLED application .
Figure 4-2 AFM images of (a) ADN and (b) MADN after heating at 95 0C for 1 hr.
Table 4-1 PL and thermal properties of ADN derivatives.
Comparison of their EL performance in an optimized device structure of ITO/CFx/NPB (70 nm)/blue host (40 nm)/Alq3 (10 nm)/LiF(1 nm)/Al (200 nm) showed that MADN had the best luminous efficiency of 1.4 cd/A and the lowest drive voltage of 6.2 V (measured at 20 mA/cm2) with also the bluest color of (0.15, 0.10) that is identical to that of TBADN, as shown in Figure 4-3(a).
Device stability data of all three nondoped devices depicted in Figure 4-3(b) confirms that MADN stands out as the best in the diarylanthracene-type of blue hosts with a projected lifetime of about 7000 hr at an initial luminance of 100
When MADN doped with the sky blue dopant,
bis[(diphenyl)aminostyryl]benzene emitter (DSA-Ph, structure is shown in Table2-1) , its EL performance can reach as high as 9.7 cd/A and 5.5 lm/W at 20 mA/cm2 with CIEx,y of (0.16, 0.32). It is believed that the high efficiency is due to the good overlap between the absorption spectrum of DSA-Ph and the emission spectrum of MADN, which is an important factor for efficient Förster energy transfer. The stability of this sky blue device is projected to be able to last for 46,000 hr at L0 = 100 cd/m2.
4.3 Development of host material for deep blue emitter
The deep-blue color is defined arbitrarily as having a blue EL emission with a CIE coordinates of y value (CIEy) < 0.15. Such an emitter can effectively reduce the power consumption of a full-color OLED and also be utilized to generate light of other colors by energy cascade to a suitable emissive dopant [33,34].
Unfortunately, literature with full disclosure on deep blue OLED dopant/host material structures is rather rare and sketchy. One notable example was by Idemitsu Kosan Co. recently presented a styrylamine-based dopant BD-3 to produce an EL efficiency of 7.2 cd/A and a blue color of (0.14, 0.16)  and likewise, Kodak also presented about one of their best deep blue devices performance with dopant BK-9 in host BH-3 which achieved an efficiency of 7.4 cd/A and a blue color of (0.14, 0.17) . Neither of them disclosed in these presentations any useful structural information that was needed to substantiate their great device performances.
In 2005, our group disclosed that MADN doped with an unsymmetrical
[4-(2-[1,1’;4’,1”]terphenyl-4-yl-vinyl)phenyl] amine (SA-BiPh), achieved an EL efficiency of 2.2 cd/A at 20 mA/cm2 with a saturated blue CIEx,y of (0.15, 0.12) and a normalized operational lifetime of 10000 hrs at an initial brightness of 100 cd/m2 .
Although SA-BiPh doped MADN emitter could achieve a saturated deep blue color, the device efficiency is still low and inadequate. It is well known that a guest–host doped emitter system can significantly improve device performance in terms of EL efficiency and emissive color .Therefore, key for developing deep blue OLEDs is not only finding the highly fluorescent deep blue dopant but also the appropriate matching host material in order to enhance the probability of carrier recombination as well as the efficiency of Förster energy-transfer from the host to the dopant molecule.
Therefore, we developed a new anthracene-based wide band gap host material, 2-methyl-9,10-di(1-napthyl)anthracene (,-MADN) in which the 2-(naphthyl)-substutuent of MADN is replaced by the sterically more demanding 1-(naphthyl)-substutient. The small methyl-substituent at C-2 position of the anthracene moiety is preserved with the purpose of disrupting the symmetry of ADN and suppressing its problematic crystallization. The thermal properties of MADN and
-MADN are summarized in Table 4-2, in whichTGA revealed that the Td of
-MADN was 397 °C. During DSCmeasurements, -MADN underwent a glass transition at a relatively high Tg
of 133 °C and also showed a high melting temperature (Tm) at 315 °C. The higher thermal properties of
-MADN, with respect to those of MADN areessential for morphological stability of thin films.
As we know, the thin-film morphological stability is very sensitive to
pin-hole formation due crystallization or any interfacial change that might be induced by Joule heating  during device operation which may in turn impact adversely on the lifetime of the device. The result of AFM measurement as shown in Figure 4-4 indicated that an evaporated film of ,-MADN possessed a uniform surface that did not undergo any morphological changes when heated at 95 °C for 1 hr. The root-mean-square surface roughness of heated ,-MADN film is 0.21 nm.
Table 4-2 Thermal, optical, and electrochemical Properties of MADN and
Figure 4-4 AFM topographic images of
-MADN thin film deposited onsilicon wafers (50 nm) after heating at 95 °C for 1 hr.
Figure 4-5 shows the absorption spectra and solution fluorescence spectra of MADN and -MADN in toluene. The band gap of -MADN is found to be 3.0 eV, which can be determined from the optical absorption threshold and is slightly larger than that of MADN (2.95 eV). In addition, it is obvious that
-MADN has a smaller stoke-shift and the fluorescence wavelength max of
-MADN is 413 nm which is blue-shifted around 17 nm with respect to thatof MADN. The principal cause of the hypsochromic-shift is most likely due to the stronger H atom-H atom repulsions between the 1-(naphthyl)-substituent and anthracene moiety of
-MADN which causes the naphthyl-group tode-conjugate from the anthracene chromophore in the ground state.
Figure 4-5 Normalized absorption and fluorescence spectra of MADN and
-MADN in toluene.
The electrochemical properties of MADN and -MADN were probed by CV as depicted in Figure 4-6. Both of MADN and
-MADN exhibitedreversible oxidation potentials (Eox) of 1.05 V and 1.12 V, respectively. On the basis of the onset potential for the oxidation and the band gap, we estimated the
HOMO and LUMO energy levels of MADN and
-MADN (see Table 4-2)with regard to the energy level of the ferrocene reference (4.8 eV below the vacuum level) .
Figure 4-6 Cyclic voltammograms of MADN and -MADN.
4.4 Energy transfer between blue host-guest materials
One of the key developments in the advancement of OLED display
One of the key developments in the advancement of OLED display